Three New Alkaline Beryllium Borates LiBeBO3, Li6Be3B4O12, and Li8Be5B6O18 in the Ternary Phase Diagrams Li2O-BeO-B2O3.
Wang, Shichao; Ye, Ning; Zou, Guohong; Inorganic chemistry 53 (2014) 2742–2748; doi:10.1021/ic5000843

data_4337787
_publ_section_title
;
 Three New Alkaline Beryllium Borates LiBeBO3, Li6Be3B4O12, and
 Li8Be5B6O18 in the Ternary Phase Diagrams Li2O-BeO-B2O3.
;
_journal_issue                   5
_journal_name_full               'Inorganic chemistry'
_journal_page_first              2742
_journal_page_last               2748
_journal_paper_doi               10.1021/ic5000843
_journal_volume                  53
_journal_year                    2014
_chemical_formula_sum            'B6 Be5 Li8 O18'
_chemical_formula_weight         453.43
_chemical_name_systematic
;
 ?
;
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                77.849(13)
_cell_angle_beta                 89.420(18)
_cell_angle_gamma                89.210(16)
_cell_formula_units_Z            2
_cell_length_a                   4.698(3)
_cell_length_b                   11.565(8)
_cell_length_c                   11.870(8)
_cell_measurement_reflns_used    1692
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.4835
_cell_measurement_theta_min      3.5115
_cell_volume                     630.4(7)
_computing_cell_refinement       'CrystalClear (Rigaku/MSC Inc., 2005)'
_computing_data_collection       'CrystalClear (Rigaku/MSC Inc., 2005)'
_computing_data_reduction        'CrystalClear (Rigaku/MSC Inc., 2005)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 14.6306
_diffrn_measured_fraction_theta_full 0.97
_diffrn_measured_fraction_theta_max 0.97
_diffrn_measurement_device
;
        Mercury70 (2x2 bin mode)
;
_diffrn_measurement_method       CCD_Profile_fitting
_diffrn_orient_matrix_type       d*Trek
_diffrn_orient_matrix_UB_11      0.2058
_diffrn_orient_matrix_UB_12      0.0527
_diffrn_orient_matrix_UB_13      -0.0134
_diffrn_orient_matrix_UB_21      0.0215
_diffrn_orient_matrix_UB_22      -0.0849
_diffrn_orient_matrix_UB_23      0.0127
_diffrn_orient_matrix_UB_31      -0.0073
_diffrn_orient_matrix_UB_32      0.0042
_diffrn_orient_matrix_UB_33      -0.0858
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0393
_diffrn_reflns_av_unetI/netI     0.0662
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            4909
_diffrn_reflns_reduction_process 'Lp corrections applied'
_diffrn_reflns_theta_full        27.51
_diffrn_reflns_theta_max         27.51
_diffrn_reflns_theta_min         2.24
_exptl_absorpt_coefficient_mu    0.21
_exptl_absorpt_correction_T_max  1
_exptl_absorpt_correction_T_min  0.4932
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            White
_exptl_crystal_density_diffrn    2.389
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Prism
_exptl_crystal_F_000             436
_exptl_crystal_size_max          0.5
_exptl_crystal_size_mid          0.1
_exptl_crystal_size_min          0.05
_refine_diff_density_max         0.451
_refine_diff_density_min         -0.386
_refine_diff_density_rms         0.095
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.209
_refine_ls_matrix_type           full
_refine_ls_number_parameters     334
_refine_ls_number_reflns         2688
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.209
_refine_ls_R_factor_all          0.0711
_refine_ls_R_factor_gt           0.0563
_refine_ls_shift/su_max          0
_refine_ls_shift/su_mean         0
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0581P)^2^+0.7991P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1637
_refine_ls_wR_factor_ref         0.1729
_reflns_number_gt                2094
_reflns_number_total             2688
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic5000843_si_002.cif
_cod_data_source_block           Li8Be5B6O18_P-1
_cod_depositor_comments
;
The following automatic conversions were performed:

'_space_group_crystal_system' value 'Triclinic' changed to
'triclinic' according to
/usr/data/users/saulius/crontab/automatic-downloads/current/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from
2011-04-26.

'_exptl_absorpt_correction_type' value 'Multi-scan'
changed to 'multi-scan' according to
/usr/data/users/saulius/crontab/automatic-downloads/current/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 
;
_cod_original_cell_volume        630.3(7)
_cod_database_code               4337787